Dye-sensitized solar cell
A dye-sensitized solar cell (DSSC, DSC, DYSC or Grätzel cell) is a low-cost solar cell belonging to the group of thin film solar cells. It is based on a semiconductor formed between a photo-sensitized anode and an electrolyte, a photoelectrochemical system. The modern version of a dye solar cell, also known as the Grätzel cell, was originally co-invented in 1988 by Brian O'Regan and Michael Grätzel at UC Berkeley and this work was later developed by the aforementioned scientists at the École Polytechnique Fédérale de Lausanne until the publication of the first high efficiency DSSC in 1991. Michael Grätzel has been awarded the 2010 Millennium Technology Prize for this invention.
The DSSC has a number of attractive features; it is simple to make using conventional roll-printing techniques, is semi-flexible and semi-transparent which offers a variety of uses not applicable to glass-based systems, and most of the materials used are low-cost. In practice it has proven difficult to eliminate a number of expensive materials, notably platinum and ruthenium, and the liquid electrolyte presents a serious challenge to making a cell suitable for use in all weather. Although its conversion efficiency is less than the best thin-film cells, in theory its price/performance ratio should be good enough to allow them to compete with fossil fuel electrical generation by achieving grid parity. Commercial applications, which were held up due to chemical stability problems, are forecast in the European Union Photovoltaic Roadmap to significantly contribute to renewable electricity generation by 2020.
- 1 Current technology: semiconductor solar cells
- 2 Dye-sensitized solar cells
- 3 Development
- 4 Market introduction
- 5 See also
- 6 References
- 7 External links
Current technology: semiconductor solar cells
In a traditional solid-state semiconductor, a solar cell is made from two doped crystals, one doped with n-type impurities (n-type semiconductor), which add additional free conduction band electrons, and the other doped with p-type impurities (p-type semiconductor), which add additional electron holes. When placed in contact, some of the electrons in the n-type portion flow into the p-type to "fill in" the missing electrons, also known as electron holes. Eventually enough electrons will flow across the boundary to equalize the Fermi levels of the two materials. The result is a region at the interface, the p-n junction, where charge carriers are depleted and/or accumulated on each side of the interface. In silicon, this transfer of electrons produces a potential barrier of about 0.6 to 0.7 V.
When placed in the sun, photons of the sunlight can excite electrons on the p-type side of the semiconductor, a process known as photoexcitation. In silicon, sunlight can provide enough energy to push an electron out of the lower-energy valence band into the higher-energy conduction band. As the name implies, electrons in the conduction band are free to move about the silicon. When a load is placed across the cell as a whole, these electrons will flow out of the p-type side into the n-type side, lose energy while moving through the external circuit, and then flow back into the p-type material where they can once again re-combine with the valence-band hole they left behind. In this way, sunlight creates an electric current.
In any semiconductor, the band gap means that only photons with that amount of energy, or more, will contribute to producing a current. In the case of silicon, the majority of visible light from red to violet has sufficient energy to make this happen. Unfortunately higher energy photons, those at the blue and violet end of the spectrum, have more than enough energy to cross the band gap; although some of this extra energy is transferred into the electrons, the majority of it is wasted as heat. Another issue is that in order to have a reasonable chance of capturing a photon, the n-type layer has to be fairly thick. This also increases the chance that a freshly ejected electron will meet up with a previously created hole in the material before reaching the p-n junction. These effects produce an upper limit on the efficiency of silicon solar cells, currently around 12 to 15% for common modules and up to 25% for the best laboratory cells (33.16% is the theoretical maximum efficiency for single band gap solar cells, see Shockley–Queisser limit.).
By far the biggest problem with the conventional approach is cost; solar cells require a relatively thick layer of doped silicon in order to have reasonable photon capture rates, and silicon processing is expensive. There have been a number of different approaches to reduce this cost over the last decade, notably the thin-film approaches, but to date they have seen limited application due to a variety of practical problems. Another line of research has been to dramatically improve efficiency through the multi-junction approach, although these cells are very high cost and suitable only for large commercial deployments. In general terms the types of cells suitable for rooftop deployment have not changed significantly in efficiency, although costs have dropped somewhat due to increased supply.
Dye-sensitized solar cells
In the late 1960s it was discovered that illuminated organic dyes can generate electricity at oxide electrodes in electrochemical cells. In an effort to understand and simulate the primary processes in photosynthesis the phenomenon was studied at the University of California at Berkeley with chlorophyll extracted from spinach (bio-mimetic or bionic approach). On the basis of such experiments electric power generation via the dye sensitization solar cell (DSSC) principle was demonstrated and discussed in 1972. The instability of the dye solar cell was identified as a main challenge. Its efficiency could, during the following two decades, be improved by optimizing the porosity of the electrode prepared from fine oxide powder, but the instability remained a problem.
A modern DSSC is composed of a porous layer of titanium dioxide nanoparticles, covered with a molecular dye that absorbs sunlight, like the chlorophyll in green leaves. The titanium dioxide is immersed under an electrolyte solution, above which is a platinum-based catalyst. As in a conventional alkaline battery, an anode (the titanium dioxide) and a cathode (the platinum) are placed on either side of a liquid conductor (the electrolyte).
Sunlight passes through the transparent electrode into the dye layer where it can excite electrons that then flow into the titanium dioxide. The electrons flow toward the transparent electrode where they are collected for powering a load. After flowing through the external circuit, they are re-introduced into the cell on a metal electrode on the back, flowing into the electrolyte. The electrolyte then transports the electrons back to the dye molecules.
Dye-sensitized solar cells separate the two functions provided by silicon in a traditional cell design. Normally the silicon acts as both the source of photoelectrons, as well as providing the electric field to separate the charges and create a current. In the dye-sensitized solar cell, the bulk of the semiconductor is used solely for charge transport, the photoelectrons are provided from a separate photosensitive dye. Charge separation occurs at the surfaces between the dye, semiconductor and electrolyte.
The dye molecules are quite small (nanometer sized), so in order to capture a reasonable amount of the incoming light the layer of dye molecules needs to be made fairly thick, much thicker than the molecules themselves. To address this problem, a nanomaterial is used as a scaffold to hold large numbers of the dye molecules in a 3-D matrix, increasing the number of molecules for any given surface area of cell. In existing designs, this scaffolding is provided by the semiconductor material, which serves double-duty.
In the case of the original Grätzel and O'Regan design, the cell has 3 primary parts. On top is a transparent anode made of fluoride-doped tin dioxide (SnO2:F) deposited on the back of a (typically glass) plate. On the back of this conductive plate is a thin layer of titanium dioxide (TiO2), which forms into a highly porous structure with an extremely high surface area. The (TiO2) is chemically bound by a process called sintering. TiO2 only absorbs a small fraction of the solar photons (those in the UV). The plate is then immersed in a mixture of a photosensitive ruthenium-polypyridine dye (also called molecular sensitizers) and a solvent. After soaking the film in the dye solution, a thin layer of the dye is left covalently bonded to the surface of the TiO2. The bond is either an ester, chelating, or bidentate bridging linkage.
A separate plate is then made with a thin layer of the iodide electrolyte spread over a conductive sheet, typically platinum metal. The two plates are then joined and sealed together to prevent the electrolyte from leaking. The construction is simple enough that there are hobby kits available to hand-construct them. Although they use a number of "advanced" materials, these are inexpensive compared to the silicon needed for normal cells because they require no expensive manufacturing steps. TiO2, for instance, is already widely used as a paint base.
One of the efficient DSSCs devices uses ruthenium-based molecular dye, e.g. [Ru(4,4'-dicarboxy-2,2'-bipyridine)2(NCS)2] (N3), that is bound to a photoanode via carboxylate moieties. The photoanode consists of 12 μm thick film of transparent 10–20 nm diameter TiO2 nanoparticles covered with a 4 μm thick film of much larger (400 nm diameter) particles that scatter photons back into the transparent film. The excited dye rapidly injects an electron into the TiO2 after light absorption. The injected electron diffuses through the sintered particle network to be collected at the front side transparent conducting oxide (TCO) electrode, while the dye is regenerated via reduction by a redox shuttle, I3/I, dissolved in a solution. Diffusion of the oxidized form of the shuttle to the counter electrode completes the circuit.
Mechanism of DSSCs
The following steps convert in a DSSC photons (light) to current:
- The incident photon is absorbed by Ru complex photosensitizers adsorbed on the TiO2 surface.
- The photosensitizers are excited from the ground state (S) to the excited state (S∗). The excited electrons are injected into the conduction band of the TiO2 electrode. This results in the oxidation of the photosensitizer (S+).
S + hν → S∗
- The injected electrons in the conduction band of TiO2 are transported between TiO2 nanoparticles with diffusion toward the back contact (TCO). And the electrons finally reach the counter electrode through the circuit.
- The oxidized photosensitizer (S+) accepts electrons from the I− ion redox mediator leading to regeneration of the ground state (S), and two I−-Ions are oxidized to elementary Iodine which reacts with I− to the oxidized state, I3−.
S+ + e− → S
- The oxidized redox mediator, I3−, diffuses toward the counter electrode and then it is reduced to I− ions.
I3− + 2 e− → 3 I−
The efficiency of a DSSC depends on four energy levels of the component: the excited state (approximately LUMO) and the ground state (HOMO) of the photosensitizer, the Fermi level of the TiO2 electrode and the redox potential of the mediator (I−/I3−) in the electrolyte.
In DSSC, electrodes consisted of sintered semiconducting nanoparticles, mainly TiO2 or ZnO. These nanoparticle DSSCs rely on trap-limited diffusion through the semiconductor nanoparticles for the electron transport. This limits the device efficiency since it is a slow transport mechanism. Recombination is more likely to occur at longer wavelengths of radiation. Moreover, sintering of nanoparticles requires a high temperature of about 450 °C, which restricts the fabrication of these cells to robust, rigid solid substrates. It has been proven that there is an increase in the efficiency of DSSC, if the sintered nanoparticle electrode is replaced by a specially designed electrode possessing an exotic 'nanoplant-like' morphology.
Sunlight enters the cell through the transparent SnO2:F top contact, striking the dye on the surface of the TiO2. Photons striking the dye with enough energy to be absorbed create an excited state of the dye, from which an electron can be "injected" directly into the conduction band of the TiO2. From there it moves by diffusion (as a result of an electron concentration gradient) to the clear anode on top.
Meanwhile, the dye molecule has lost an electron and the molecule will decompose if another electron is not provided. The dye strips one from iodide in electrolyte below the TiO2, oxidizing it into triiodide. This reaction occurs quite quickly compared to the time that it takes for the injected electron to recombine with the oxidized dye molecule, preventing this recombination reaction that would effectively short-circuit the solar cell.
The triiodide then recovers its missing electron by mechanically diffusing to the bottom of the cell, where the counter electrode re-introduces the electrons after flowing through the external circuit.
Several important measures are used to characterize solar cells. The most obvious is the total amount of electrical power produced for a given amount of solar power shining on the cell. Expressed as a percentage, this is known as the solar conversion efficiency. Electrical power is the product of current and voltage, so the maximum values for these measurements are important as well, Jsc and Voc respectively. Finally, in order to understand the underlying physics, the "quantum efficiency" is used to compare the chance that one photon (of a particular energy) will create one electron.
In quantum efficiency terms, DSSCs are extremely efficient. Due to their "depth" in the nanostructure there is a very high chance that a photon will be absorbed, and the dyes are very effective at converting them to electrons. Most of the small losses that do exist in DSSC's are due to conduction losses in the TiO2 and the clear electrode, or optical losses in the front electrode. The overall quantum efficiency for green light is about 90%, with the "lost" 10% being largely accounted for by the optical losses in the top electrode. The quantum efficiency of traditional designs vary, depending on their thickness, but are about the same as the DSSC.
In theory, the maximum voltage generated by such a cell is simply the difference between the (quasi-)Fermi level of the TiO2 and the redox potential of the electrolyte, about 0.7 V under solar illumination conditions (Voc). That is, if an illuminated DSSC is connected to a voltmeter in an "open circuit", it would read about 0.7 V. In terms of voltage, DSSCs offer slightly higher Voc than silicon, about 0.7 V compared to 0.6 V. This is a fairly small difference, so real-world differences are dominated by current production, Jsc.
Although the dye is highly efficient at converting absorbed photons into free electrons in the TiO2, only photons absorbed by the dye ultimately produce current. The rate of photon absorption depends upon the absorption spectrum of the sensitized TiO2 layer and upon the solar flux spectrum. The overlap between these two spectra determines the maximum possible photocurrent. Typically used dye molecules generally have poorer absorption in the red part of the spectrum compared to silicon, which means that fewer of the photons in sunlight are usable for current generation. These factors limit the current generated by a DSSC, for comparison, a traditional silicon-based solar cell offers about 35 mA/cm2, whereas current DSSCs offer about 20 mA/cm2.
DSSCs degrade when exposed to ultraviolet radiation. In 2014 air infiltration of the commonly-used amorphous Spiro-MeOTAD hole-transport layer was identified as the primary cause of the degradation, rather than oxidation. The damage could be avoided by the addition of an appropriate barrier.
The barrier layer may include UV stabilizers and/or UV absorbing luminescent chromophores (which emit at longer wavelengths which may be reabsorbed by the dye) and antioxidants to protect and improve the efficiency of the cell.
DSSCs are currently the most efficient third-generation (2005 Basic Research Solar Energy Utilization 16) solar technology available. Other thin-film technologies are typically between 5% and 13%, and traditional low-cost commercial silicon panels operate between 14% and 17%. This makes DSSCs attractive as a replacement for existing technologies in "low density" applications like rooftop solar collectors, where the mechanical robustness and light weight of the glass-less collector is a major advantage. They may not be as attractive for large-scale deployments where higher-cost higher-efficiency cells are more viable, but even small increases in the DSSC conversion efficiency might make them suitable for some of these roles as well.
There is another area where DSSCs are particularly attractive. The process of injecting an electron directly into the TiO2 is qualitatively different from that occurring in a traditional cell, where the electron is "promoted" within the original crystal. In theory, given low rates of production, the high-energy electron in the silicon could re-combine with its own hole, giving off a photon (or other form of energy) which does not result in current being generated. Although this particular case may not be common, it is fairly easy for an electron generated by another atom to combine with a hole left behind in a previous photoexcitation.
In comparison, the injection process used in the DSSC does not introduce a hole in the TiO2, only an extra electron. Although it is energetically possible for the electron to recombine back into the dye, the rate at which this occurs is quite slow compared to the rate that the dye regains an electron from the surrounding electrolyte. Recombination directly from the TiO2 to species in the electrolyte is also possible although, again, for optimized devices this reaction is rather slow. On the contrary, electron transfer from the platinum coated electrode to species in the electrolyte is necessarily very fast.
As a result of these favorable "differential kinetics", DSSCs work even in low-light conditions. DSSCs are therefore able to work under cloudy skies and non-direct sunlight, whereas traditional designs would suffer a "cutout" at some lower limit of illumination, when charge carrier mobility is low and recombination becomes a major issue. The cutoff is so low they are even being proposed for indoor use, collecting energy for small devices from the lights in the house.
A practical advantage which DSSCs share with most thin-film technologies, is that the cell's mechanical robustness indirectly leads to higher efficiencies at higher temperatures. In any semiconductor, increasing temperature will promote some electrons into the conduction band "mechanically". The fragility of traditional silicon cells requires them to be protected from the elements, typically by encasing them in a glass box similar to a greenhouse, with a metal backing for strength. Such systems suffer noticeable decreases in efficiency as the cells heat up internally. DSSCs are normally built with only a thin layer of conductive plastic on the front layer, allowing them to radiate away heat much easier, and therefore operate at lower internal temperatures.
The major disadvantage to the DSSC design is the use of the liquid electrolyte, which has temperature stability problems. At low temperatures the electrolyte can freeze, halting power production and potentially leading to physical damage. Higher temperatures cause the liquid to expand, making sealing the panels a serious problem. Another disadvantage is that costly ruthenium (dye), platinum (catalyst) and conducting glass or plastic (contact) are needed to produce a DSSC. A third major drawback is that the electrolyte solution contains volatile organic compounds (or VOC's), solvents which must be carefully sealed as they are hazardous to human health and the environment. This, along with the fact that the solvents permeate plastics, has precluded large-scale outdoor application and integration into flexible structure.
Replacing the liquid electrolyte with a solid has been a major ongoing field of research. Recent experiments using solidified melted salts have shown some promise, but currently suffer from higher degradation during continued operation, and are not flexible.
Photocathodes and tandem cells
Dye sensitised solar cells operate as a photoanode (n-DSC), where photocurrent result from electron injection by the sensitized dye. Photocathodes (p-DSCs) operate in an inverse mode compared to the conventional n-DSC, where dye-excitation is followed by rapid electron transfer from a p-type semiconductor to the dye (dye-sensitized hole injection, instead of electron injection). Such p-DSCs and n-DSCs can be combined to construct tandem solar cells (pn-DSCs) and the theoretical efficiency of tandem DSCs is well beyond that of single-junction DSCs.
A standard tandem cell consists of one n-DSC and one p-DSC in a simple sandwich configuration with an intermediate electrolyte layer. n-DSC and p-DSC are connected in series, which implies that the resulting photocurrent will be controlled by the weakest photoelectrode, whereas photovoltages are additive. Thus, photocurrent matching is very important for the construction of highly efficient tandem pn-DSCs. However, unlike n-DSCs, fast charge recombination following dye-sensitized hole injection usually resulted in low photocurrents in p-DSC and thus hampered the efficiency of the overall device.
Researchers have found that using dyes comprising a perylenemonoimide (PMI) as the acceptor and an oligothiophene coupled to triphenylamine as the donor greatly improve the performance of p-DSC by reducing charge recombination rate following dye-sensitized hole injection. The researchers constructed a tandem DSC device with NiO on the p-DSC side and TiO2 on the n-DSC side. Photocurrent matching was achieved through adjustment of NiO and TiO2 film thicknesses to control the optical absorptions and therefore match the photocurrents of both electrodes. The energy conversion efficiency of the device is 1.91%, which exceeds the efficiency of its individual components, but is still much lower than that of high performance n-DSC devices (6%–11%). The results are still promising since the tandem DSC was in itself rudimentary. The dramatic improvement in performance in p-DSC can eventually lead to tandem devices with much greater efficiency than lone n-DSCs.
Using electron transporting materials such as PCBM, TiO2 and ZnO instead of the conventional liquid redox couple electrolyte, researchers have managed to fabricate the solid state p-DSC (p-ssDSCs), aiming for solid state tandem dye sensitized solar cells.
The dyes used in early experimental cells (circa 1995) were sensitive only in the high-frequency end of the solar spectrum, in the UV and blue. Newer versions were quickly introduced (circa 1999) that had much wider frequency response, notably "triscarboxy-ruthenium terpyridine" [Ru(4,4',4"-(COOH)3-terpy)(NCS)3], which is efficient right into the low-frequency range of red and IR light. The wide spectral response results in the dye having a deep brown-black color, and is referred to simply as "black dye". The dyes have an excellent chance of converting a photon into an electron, originally around 80% but improving to almost perfect conversion in more recent dyes, the overall efficiency is about 90%, with the "lost" 10% being largely accounted for by the optical losses in top electrode.
A solar cell must be capable of producing electricity for at least twenty years, without a significant decrease in efficiency (life span). The "black dye" system was subjected to 50 million cycles, the equivalent of ten years' exposure to the sun in Switzerland. No discernible performance decrease was observed. However the dye is subject to breakdown in high-light situations. Over the last decade an extensive research program has been carried out to address these concerns. The newer dyes included 1-ethyl-3 methylimidazolium tetrocyanoborate [EMIB(CN)4] which is extremely light- and temperature-stable, copper-diselenium [Cu(In,GA)Se2] which offers higher conversion efficiencies, and others with varying special-purpose properties.
DSSCs are still at the start of their development cycle. Efficiency gains are possible and have recently started more widespread study. These include the use of quantum dots for conversion of higher-energy (higher frequency) light into multiple electrons, using solid-state electrolytes for better temperature response, and changing the doping of the TiO2 to better match it with the electrolyte being used.
A group of researchers at the Swiss Federal Institute of Technology has reportedly increased the thermostability of DSC by using amphiphilic ruthenium sensitizer in conjunction with quasi-solid-state gel electrolyte. The stability of the device matches that of a conventional inorganic silicon-based solar cell. The cell sustained heating for 1,000 h at 80 °C.
The group has previously prepared a ruthenium amphiphilic dye Z-907 (cis-Ru(H2dcbpy)(dnbpy)(NCS)2, where the ligand H2dcbpy is 4,4′-dicarboxylic acid-2,2′-bipyridine and dnbpy is 4,4′-dinonyl-2,2′-bipyridine) to increase dye tolerance to water in the electrolytes. In addition, the group also prepared a quasi-solid-state gel electrolyte with a 3-methoxypropionitrile (MPN)-based liquid electrolyte that was solidified by a photochemically stable fluorine polymer, polyvinylidenefluoride-co-hexafluoropropylene (PVDF-HFP).
The use of the amphiphilic Z-907 dye in conjunction with the polymer gel electrolyte in DSC achieved an energy conversion efficiency of 6.1%. More importantly, the device was stable under thermal stress and soaking with light. The high conversion efficiency of the cell was sustained after heating for 1,000 h at 80 °C, maintaining 94% of its initial value. After accelerated testing in a solar simulator for 1,000 h of light-soaking at 55 °C (100 mW cm−2) the efficiency had decreased by less than 5% for cells covered with an ultraviolet absorbing polymer film. These results are well within the limit for that of traditional inorganic silicon solar cells.
The enhanced performance may arise from a decrease in solvent permeation across the sealant due to the application of the polymer gel electrolyte. The polymer gel electrolyte is quasi-solid at room temperature, and becomes a viscous liquid (viscosity: 4.34 mPa·s) at 80 °C compared with the traditional liquid electrolyte (viscosity: 0.91 mPa·s). The much improved stabilities of the device under both thermal stress and soaking with light has never before been seen in DSCs, and they match the durability criteria applied to solar cells for outdoor use, which makes these devices viable for practical application.
The first successful solid-hybrid dye-sensitized solar cells were reported.
To improve electron transport in these solar cells, while maintaining the high surface area needed for dye adsorption, two researchers have designed alternate semiconductor morphologies, such as arrays of nanowires and a combination of nanowires and nanoparticles, to provide a direct path to the electrode via the semiconductor conduction band. Such structures may provide a means to improve the quantum efficiency of DSSCs in the red region of the spectrum, where their performance is currently limited.
On August 2006, to prove the chemical and thermal robustness of the 1-ethyl-3 methylimidazolium tetracyanoborate solar cell, the researchers subjected the devices to heating at 80 °C in the dark for 1000 hours, followed by light soaking at 60 °C for 1000 hours. After dark heating and light soaking, 90% of the initial photovoltaic efficiency was maintained – the first time such excellent thermal stability has been observed for a liquid electrolyte that exhibits such a high conversion efficiency. Contrary to silicon solar cells, whose performance declines with increasing temperature, the dye-sensitized solar-cell devices were only negligibly influenced when increasing the operating temperature from ambient to 60 °C.
Wayne Campbell at Massey University, New Zealand, has experimented with a wide variety of organic dyes based on porphyrin. In nature, porphyrin is the basic building block of the hemoproteins, which include chlorophyll in plants and hemoglobin in animals. He reports efficiency on the order of 5.6% using these low-cost dyes.
An article published in Nature Materials demonstrated cell efficiencies of 8.2% using a new solvent-free liquid redox electrolyte consisting of a melt of three salts, as an alternative to using organic solvents as an electrolyte solution. Although the efficiency with this electrolyte is less than the 11% being delivered using the existing iodine-based solutions, the team is confident the efficiency can be improved.
A group of researchers at Georgia Tech made dye-sensitized solar cells with a higher effective surface area by wrapping the cells around a quartz optical fiber. The researchers removed the cladding from optical fibers, grew zinc oxide nanowires along the surface, treated them with dye molecules, surrounded the fibers by an electrolyte and a metal film that carries electrons off the fiber. The cells are six times more efficient than a zinc oxide cell with the same surface area. Photons bounce inside the fiber as they travel, so there are more chances to interact with the solar cell and produce more current. These devices only collect light at the tips, but future fiber cells could be made to absorb light along the entire length of the fiber, which would require a coating that is conductive as well as transparent. Max Shtein of the University of Michigan said a sun-tracking system would not be necessary for such cells, and would work on cloudy days when light is diffuse.
- "New molecules" have been created for the electrolyte, resulting in a liquid or gel that is transparent and non-corrosive, which can increase the photovoltage and improve the cell's output and stability.
- At the cathode, platinum was replaced by cobalt sulfide, which is far less expensive, more efficient, more stable and easier to produce in the laboratory.
Dyesol and CSIRO announced in October a Successful Completion of Second Milestone in Joint Dyesol / CSIRO Project. Dyesol Director Gordon Thompson said, "The materials developed during this joint collaboration have the potential to significantly advance the commercialisation of DSC in a range of applications where performance and stability are essential requirements. Dyesol is extremely encouraged by the breakthroughs in the chemistry allowing the production of the target molecules. This creates a path to the immediate commercial utilisation of these new materials."
Dyesol and Tata Steel Europe announced in November the targeted development of Grid Parity Competitive BIPV solar steel that does not require government subsidised feed in tariffs. TATA-Dyesol "Solar Steel" Roofing is currently being installed on the Sustainable Building Envelope Centre (SBEC) in Shotton, Wales.
Northwestern University researchers announced a solution to a primary problem of DSSCs, that of difficulties in using and containing the liquid electrolyte and the consequent relatively short useful life of the device. This is achieved through the use of nanotechnology and the conversion of the liquid electrolyte to a solid. The current efficiency is about half that of silicon cells, but the cells are lightweight and potentially of much lower cost to produce.
During the last 5–10 years, a new kind of DSSC has been developed — the solid state dye-sensitized solar cell. In this case the liquid electrolyte is replaced by one of several solid hole conducting materials. From 2009 to 2013 the efficiency of Solid State DSSCs has dramatically increased from 4% to 15%. Michael Grätzel announced the fabrication of Solid State DSSCs with 15.0% efficiency, reached by the means of a hybrid perovskite CH3NH3PbI3 dye, subsequently deposited from the separated solutions of CH3NH3I and PbI2.
The first architectural integration was demonstrated at EPFL's new convention center in partnership with Romande Energie. The total surface is 300 m2, in 1400 modules of 50 cm x 35 cm. Designed by artists Daniel Schlaepfer and Catherine Bolle.
Researchers have investigated the role of surface plasmon resonances present on gold nanorods in the performance of dye-sensitized solar cells. They found that with an increase nanorod concentration, the light absorption grew linearly; however, charge extraction was also dependent on the concentration. With an optimized concentration, they found that the overall power conversion efficiency improved from 5.31 to 8.86% for Y123 dye-sensitized solar cells.
The synthesis of one-dimensional TiO2 nanostructures directly on fluorine-doped tin oxide glass substrates was successful demonstrated via a two-stop solvothermal reaction. Additionally, through a TiO2 sol treatment, the performance of the dual TiO2 nanowire cells was enhanced, reaching a power conversion efficiency of 7.65%.
Stainless steel based counter-electrodes for DSSCs have been reported which further reduce cost compared to conventional platinum based counter electrode and are suitable for outdoor application.
Researchers from EPFL have advanced the DSSCs based on copper complexes redox electrolytes, which have achieved 13.1% efficiency under standard AM1.5G, 100 mW/cm2 conditions and record 32% efficiency under 1000 lux of indoor light.
Several commercial providers are promising availability of DSCs in the near future:
- Dyesol officially opened its new manufacturing facilities in Queanbeyan Australia on 7 October 2008. It has subsequently announced partnerships with Tata Steel (TATA-Dyesol) and Pilkington Glass (Dyetec-Solar) for the development and large scale manufacture of DSC BIPV. Dyesol has also entered working relationships with Merck, Umicore, CSIRO, Japanese Ministry of Economy and Trade, Singapore Aerospace Manufacturing and a joint Venture with TIMO Korea (Dyesol-TIMO).
- Solaronix, a Swiss company specialized in the production of DSC materials since 1993, has extended their premises in 2010 to host a manufacturing pilot line of DSC modules.
- SolarPrint was founded in Ireland in 2008 by Dr. Mazhar Bari, Andre Fernon and Roy Horgan. SolarPrint was the first Ireland-based commercial entity involved in the manufacturing of PV technology. SolarPrint's innovation was the solution to the solvent-based electrolyte which to date has prohibited the mass commercialisation of DSSC. The company went into receivership in 2014 and was wound up.
- G24innovations founded in 2006, based in Cardiff, South Wales, UK. On 17 October 2007, claimed the production of the first commercial grade dye sensitised thin films.
- Sony Corporation has developed dye-sensitized solar cells with an energy conversion efficiency of 10%, a level seen as necessary for commercial use.
- Tasnee Enters Strategic Investment Agreement with Dyesol.
- H.Glass was founded 2011 in Switzerland. H.Glass has put enormous efforts to create industrial process for the DSSC technologie - the first results where shown at the EXPO 2015 in Milano at the Austrian Pavilion. The milestone for DSSC is the Science Tower in Austria - it is the largest installation of DSSC in the world - carried out by SFL technologies.
- Wan, Haiying "Dye Sensitized Solar Cells", University of Alabama Department of Chemistry, p. 3
- "Dye-Sensitized vs. Thin Film Solar Cells", European Institute for Energy Research, 30 June 2006
- EarlyHistory. Workspace.imperial.ac.uk. Retrieved on 30 May 2013.
- O'Regan, Brian; Grätzel, Michael (1991). "A low-cost, high-efficiency solar cell based on dye-sensitized colloidal TiO2 films". Nature. 353 (6346): 737–40. Bibcode:1991Natur.353..737O. doi:10.1038/353737a0.
- Professor Grätzel wins the 2010 millennium technology grand prize for dye-sensitized solar cells, Technology Academy Finland, 14 June 2010.
- Tributsch, H (2004). "Dye sensitization solar cells: A critical assessment of the learning curve". Coordination Chemistry Reviews. 248 (13–14): 1511–30. doi:10.1016/j.ccr.2004.05.030.
- "Photovoltaic Cells (Solar Cells), How They Work". specmat.com. Retrieved 22 May 2007.
- Rühle, Sven (2016). "Tabulated values of the Shockley–Queisser limit for single junction solar cells". Solar Energy. 130: 139–47. Bibcode:2016SoEn..130..139R. doi:10.1016/j.solener.2016.02.015.
- Gerischer, H; Michel-Beyerle, M.E; Rebentrost, F; Tributsch, H (1968). "Sensitization of charge injection into semiconductors with large band gap". Electrochimica Acta. 13 (6): 1509–15. doi:10.1016/0013-4686(68)80076-3.
- Tributsch, H; Calvin, M (1971). "Electrochemistry of Excited Molecules: Photo-Electrochemical Reactions of Chlorophylls". Photochemistry and Photobiology. 14 (2): 95–112. doi:10.1111/j.1751-1097.1971.tb06156.x.
- Tributsch, Helmut (2008). "Reaction of Excited Chlorophyll Molecules at Electrodes and in Photosynthesis". Photochemistry and Photobiology. 16 (4): 261–9. doi:10.1111/j.1751-1097.1972.tb06297.x.
- Matsumura, Michio; Matsudaira, Shigeyuki; Tsubomura, Hiroshi; Takata, Masasuke; Yanagida, Hiroaki (1980). "Dye Sensitization and Surface Structures of Semiconductor Electrodes". Industrial & Engineering Chemistry Product Research and Development. 19 (3): 415–21. doi:10.1021/i360075a025.
- Juan Bisquert, "Dye-sensitized solar cells", Departament de Física, Universitat Jaume I
- "Dye Solar Cell Assembly Instructions". Solaronix. Archived from the original on 28 September 2007. Retrieved 22 May 2007.
- Hamann, Thomas W; Jensen, Rebecca A; Martinson, Alex B. F; Van Ryswyk, Hal; Hupp, Joseph T (2008). "Advancing beyond current generation dye-sensitized solar cells". Energy & Environmental Science. 1: 66–78. doi:10.1039/b809672d.
- Hara, Kohjiro; Arakawa, Hironori (2005). "Dye-Sensitized Solar Cells". Handbook of Photovoltaic Science and Engineering. pp. 663–700. doi:10.1002/0470014008.ch15. ISBN 9780470014004.
- Tiwari, Ashutosh; Snure, Michael (2008). "Synthesis and Characterization of ZnO Nano-Plant-Like Electrodes". Journal of Nanoscience and Nanotechnology. 8 (8): 3981–7. doi:10.1166/jnn.2008.299. PMID 19049161.
- American Chemical Society, "Ultrathin, Dye-sensitized Solar Cells Called Most Efficient To Date", ScienceDaily, 20 September 2006
- Gao, Feifei; Wang, Yuan; Zhang, Jing; Shi, Dong; Wang, Mingkui; Humphry-Baker, Robin; Wang, Peng; Zakeeruddin, Shaik M; Grätzel, Michael (2008). "A new heteroleptic ruthenium sensitizer enhances the absorptivity of mesoporous titania film for a high efficiency dye-sensitized solar cell". Chemical Communications (23): 2635–7. doi:10.1039/b802909a. PMID 18535691.
- press release of EPFL
- Burschka, Julian; Pellet, Norman; Moon, Soo-Jin; Humphry-Baker, Robin; Gao, Peng; Nazeeruddin, Mohammad K; Grätzel, Michael (2013). "Sequential deposition as a route to high-performance perovskite-sensitized solar cells". Nature. 499 (7458): 316–9. Bibcode:2013Natur.499..316B. doi:10.1038/nature12340. PMID 23842493.
- Estes, Kathleen (7 April 2014). "New findings to help extend high efficiency solar cells' lifetime". Rdmag.com. Retrieved 24 August 2014.
- Chittibabu, Kethinni, G. et al. Photovoltaic cell, European patent WO/2004/006292, Publication Date: 15 January 2004.
- Basic Research Needs for Solar Energy Utilization, U.S. Department of Energy Office of Basic Energy Sciences, 2005.
- Jessica Krüger, "Interface engineering in solid-state dye sensitized solar cells", École Polytechnique Fédérale de Lausanne, 2003
- Kimberly Patch, "Solar cell doubles as battery", Technology Research News, 2006
- Ecole Polytechnique Fédérale de Lausanne, "New Efficiency Benchmark For Dye-sensitized Solar Cells", ScienceDaily, 3 November 2008
- Nathalie Rossier-Iten, "Solid hybrid dye-sensitized solar cells: new organic materials, charge recombination and stability", École Polytechnique Fédérale de Lausanne, 2006
- Nattestad, A; Mozer, A. J; Fischer, M. K. R; Cheng, Y.-B; Mishra, A; Bäuerle, P; Bach, U (2009). "Highly efficient photocathodes for dye-sensitized tandem solar cells". Nature Materials. 9 (1): 31–5. Bibcode:2010NatMa...9...31N. doi:10.1038/nmat2588. PMID 19946281.
- Tian, Haining; Hammarström, Leif; Boschloo, Gerrit; Zhang, Lei (10 February 2016). "Solid state p-type dye-sensitized solar cells: concept, experiment and mechanism". Physical Chemistry Chemical Physics. 18 (7): 5080–5085. doi:10.1039/C5CP05247E. ISSN 1463-9084.
- Tian, Haining; Hammarström, Leif; Boschloo, Gerrit; Sun, Junliang; Kubart, Tomas; Johansson, Malin; Yang, Wenxing; Lin, Junzhong; Zhang, Zhibin (20 December 2017). "Ultrafast dye regeneration in a core–shell NiO–dye–TiO2 mesoporous film". Physical Chemistry Chemical Physics. 20 (1): 36–40. doi:10.1039/C7CP07088H. ISSN 1463-9084.
- Tian, Haining; Hammarström, Leif; Boschloo, Gerrit; Kloo, Lars; Sun, Junliang; Hua, Yong; Kubart, Tomas; Lin, Junzhong; Pati, Palas Baran (10 April 2018). "Solid state p-type dye sensitized NiO–dye–TiO2 core–shell solar cells". Chemical Communications. 54 (30): 3739–3742. doi:10.1039/C8CC00505B. ISSN 1364-548X.
- "ScienceDirect". www.sciencedirect.com. Retrieved 6 May 2019.
- Tian, Haining (26 March 2019). "Solid-state p-type dye-sensitized solar cells: progress, potential applications and challenges". Sustainable Energy & Fuels. 3 (4): 888–898. doi:10.1039/C8SE00581H. ISSN 2398-4902.
- Kalyanasundaram, K.; Grätzel, Michael (2 February 1999). "Dye Sensitized Solar Cells (DYSC) based on Nanocrystalline Oxide Semiconductor Films". Laboratory for Photonics and Interfaces, École Polytechnique Fédérale de Lausanne. Archived from the original on 6 February 2005. Retrieved 22 May 2007.
- Wang, Peng; Zakeeruddin, Shaik M; Moser, Jacques E; Nazeeruddin, Mohammad K; Sekiguchi, Takashi; Grätzel, Michael (2003). "A stable quasi-solid-state dye-sensitized solar cell with an amphiphilic ruthenium sensitizer and polymer gel electrolyte". Nature Materials. 2 (6): 402–7. Bibcode:2003NatMa...2..402W. doi:10.1038/nmat904. PMID 12754500.
- Grätzel, Michael (2003). "Dye-sensitized solar cells". Journal of Photochemistry and Photobiology C: Photochemistry Reviews. 4 (2): 145–53. doi:10.1016/S1389-5567(03)00026-1.
- Michael Berger, "Nanowires Could Lead to Improved Solar Cells ", NewswireToday, 03/06/2006
- Campbell, Wayne M; Jolley, Kenneth W; Wagner, Pawel; Wagner, Klaudia; Walsh, Penny J; Gordon, Keith C; Schmidt-Mende, Lukas; Nazeeruddin, Mohammad K; Wang, Qing; Grätzel, Michael; Officer, David L (2007). "Highly Efficient Porphyrin Sensitizers for Dye-Sensitized Solar Cells". The Journal of Physical Chemistry C. 111 (32): 11760–2. CiteSeerX 10.1.1.459.6793. doi:10.1021/jp0750598.
- Wang, Qing; Campbell, Wayne M; Bonfantani, Edia E; Jolley, Kenneth W; Officer, David L; Walsh, Penny J; Gordon, Keith; Humphry-Baker, Robin; Nazeeruddin, Mohammad K; Grätzel, Michael (2005). "Efficient Light Harvesting by Using Green Zn-Porphyrin-Sensitized Nanocrystalline TiO2Films". The Journal of Physical Chemistry B. 109 (32): 15397–409. doi:10.1021/jp052877w. PMID 16852953.
- Bai, Yu; Cao, Yiming; Zhang, Jing; Wang, Mingkui; Li, Renzhi; Wang, Peng; Zakeeruddin, Shaik M; Grätzel, Michael (2008). "High-performance dye-sensitized solar cells based on solvent-free electrolytes produced from eutectic melts". Nature Materials. 7 (8): 626–30. Bibcode:2008NatMa...7..626B. doi:10.1038/nmat2224. PMID 18587401.
- Bourzac, Katherine (30 October 2009). "Wrapping Solar Cells around an Optical Fiber". Technology Review. Retrieved 31 October 2009.
- Weintraub, Benjamin; Wei, Yaguang; Wang, Zhong Lin (2009). "Optical Fiber/Nanowire Hybrid Structures for Efficient Three-Dimensional Dye-Sensitized Solar Cells". Angewandte Chemie International Edition. 48 (47): 8981–5. doi:10.1002/anie.200904492. PMID 19852015.
- Coxworth, Ben (8 April 2010) Breakthrough in low-cost efficient solar cells, Gizmag.
- Inexpensive Highly Efficient Solar Cells Possible, ScienceDaily, 12 April 2010.
- Tata Steel and Dyesol produce world’s largest dye sensitised photovoltaic module. Tatasteeleurope.com (10 June 2011). Retrieved on 26 July 2011.
- Dye-sensitized solar cell. Dyesol (21 October 2011). Retrieved on 6 January 2012.
- Industrialisation Target Confirmed. Dyesol. 21 November 2011
- DYESOL LIMITED – Dyesol 2011 AGM – Boardroom Radio webcast. Brr.com.au (23 November 2011). Retrieved on 6 January 2012.
- Taking Solar Technology Up a Notch (Northwestern University, Wednesday 23 May 2012)
- EPFL's campus has the world's first solar window
- Chandrasekhar, P. S; Parashar, Piyush K; Swami, Sanjay Kumar; Dutta, Viresh; Komarala, Vamsi K (2018). "Enhancement of Y123 dye-sensitized solar cell performance using plasmonic gold nanorods". Physical Chemistry Chemical Physics. 20 (14): 9651–8. Bibcode:2018PCCP...20.9651C. doi:10.1039/C7CP08445E.
- Kartikay, Purnendu; Nemala, Siva Sankar; Mallick, Sudhanshu (2017). "One-dimensional TiO2 nanostructured photoanode for dye-sensitized solar cells by hydrothermal synthesis". Journal of Materials Science: Materials in Electronics. 28 (15): 11528–33. doi:10.1007/s10854-017-6950-2.
- Liu, Yi-Yi; Ye, Xin-Yu; An, Qing-Qing; Lei, Bing-Xin; Sun, Wei; Sun, Zhen-Fan (2018). "A novel synthesis of the bottom-straight and top-bent dual TiO 2 nanowires for dye-sensitized solar cells". Advanced Powder Technology. 29 (6): 1455–62. doi:10.1016/j.apt.2018.03.008.
- Nemala, Siva Sankar; Kartikay, Purnendu; Agrawal, Rahul Kumar; Bhargava, Parag; Mallick, Sudhanshu; Bohm, Sivasambu (2018). "Few layers graphene based conductive composite inks for Pt free stainless steel counter electrodes for DSSC". Solar Energy. 169: 67–74. Bibcode:2018SoEn..169...67N. doi:10.1016/j.solener.2018.02.061.
- Li, Heng; Zhao, Qing; Dong, Hui; Ma, Qianli; Wang, Wei; Xu, Dongsheng; Yu, Dapeng (2014). "Highly-flexible, low-cost, all stainless steel mesh-based dye-sensitized solar cells". Nanoscale. 6 (21): 13203–12. Bibcode:2014Nanos...613203L. doi:10.1039/C4NR03999H. PMID 25254313.
- Cao, Yiming; Liu, Yuhang; Zakeeruddin, Shaik Mohammed; Hagfeldt, Anders; Grätzel, Michael (2018). "Direct Contact of Selective Charge Extraction Layers Enables High-Efficiency Molecular Photovoltaics". Joule. 2 (6): 1108–1117. doi:10.1016/j.joule.2018.03.017.
- Service, Robert F (2018). "Solar cells that work in low light could charge devices indoors". Science. doi:10.1126/science.aat9682.
- "ScienceDirect". www.sciencedirect.com. Retrieved 6 May 2019.
- Tian, Haining; Hammarström, Leif; Boschloo, Gerrit; Kloo, Lars; Sun, Junliang; Hua, Yong; Kubart, Tomas; Lin, Junzhong; Pati, Palas Baran (10 April 2018). "Solid state p-type dye sensitized NiO–dye–TiO2 core–shell solar cells". Chemical Communications. 54 (30): 3739–3742. doi:10.1039/C8CC00505B. ISSN 1364-548X.
- Gonçalves, Luís Moreira; De Zea Bermudez, Verónica; Ribeiro, Helena Aguilar; Mendes, Adélio Magalhães (2008). "Dye-sensitized solar cells: A safe bet for the future". Energy & Environmental Science. 1 (6): 655–67. doi:10.1039/b807236a.
- Company announcements for DYESOL LIMITED (DYE) Released between 01/01/2010 and 31/12/2010. Asx.com.au. Retrieved on 6 January 2012.
- Company announcements for DYESOL LIMITED (DYE) Released between 01/01/2009 and 31/12/2009. Asx.com.au. Retrieved on 6 January 2012.
- "Solaronix announces expansion", 27 January 2010.
- Ionic Liquids. basionics.com, November 2008.
- world’s first. G24i.com (17 October 2007). Retrieved on 26 July 2011.
- LATEST: Tasnee Enters Strategic Investment Agreement with Dyesol. Retrieved on 28 March 2013.
|Wikimedia Commons has media related to Dye-sensitized solar cell.|
- Brian O'Regan's account of the invention of the modern DSSC
- Dye Solar Cells for Real, the assembly guide for making your own solar cells
- Breakthrough in low-cost efficient solar cells
- DSSC Manual (National Science Foundation)
- How to Build Your Own Solar Cell, A Nanocrystalline Dye-Sensitized Solar Cell (DIY)
- Global picture for dye-sensitized solar cells.
- Cao, Guozhong (18 September 2008). "Popcorn-style dye-sensitized solar cells". SPIE.
- Solar Cells for Cheap – 2006 interview with the inventor Michael Grätzel at TechnologyReview
- Taking nature’s cue for cheaper solar power Wayne Campbell's research on using Porphyrin for highly efficient cells
- "What is the Fill Factor Of A Solar Cell?". SolarFreaks.
- What on earth is a Grätzel solar cell, and why is it so important? Interview with Dr Wayne Campbell broadcast 21 April 2007
- Simonite, Tom (19 December 2007). "Carbon electrodes could slash cost of solar panels". New Scientist.
- Lenzmann, F. O; Kroon, J. M (2007). "Recent Advances in Dye-Sensitized Solar Cells". Advances in OptoElectronics. 2007: 1–10. doi:10.1155/2007/65073.
- "Ultrathin, Dye-sensitized Solar Cells Called Most Efficient To Date". Science Daily. 20 September 2006.
- "Taking Nature's Cue For Cheaper Solar Power". Science Daily. 6 April 2007.